is a kind of heat resistant stainless steel, which is widely used as the material of aeroturbine blades owing to its generally outstanding mechanical property such as excellent toughness, oxidation resistance and corrosion resistance. Since strict requirements of geometric accuracy and surface quality have to be fulfilled, grinding process is always applied as the final finishing of the blades .Unfortunately, mechanical properties of high temperature stainless steel 1Cr11Ni2W2MoV
make it difficult to grind and may lead to elevated temperatures at the grinding zone and possible grinding burn on surface of the workpiece during grinding with abrasive wheels, which deteriorate the surface quality of the workpiece seriously. Extensive research has been carried out on the surface integrity when grinding high temperature alloy and titanium alloys [2-5], and few studies on grinding burn mechanism of stainless steel was reported. Demands on reducing the grinding costs and increasing grinding efficiency have been posing continuous challenges for the high temperature stainless steel’ grinding technologies. The sol-gel alumina abrasive wheel is a new type of grinding wheel developed in recent years. There have been no profound studies reported on the grinding characteristic of high temperature stainless steel with SG wheels.
Carbon C: 0.10~0.16
Silicon Si: ≤0.60
Manganese Mn: ≤0.60
Sulfur S :≤0.030
Phosphorus P :≤0.035
Chromium Cr: 10.50~12.00
Nickel Ni: 1.40~1.80
Vanadium V: 0.18~0.30
Molybdenum Mo: 0.35~0.50
Tungsten W: 1.50~2.00
Tensile strength σb (MPa): 1) ≥ 885; 2) ≥ 1080
Conditional yield strength σ0.2 (MPa): 1) ≥ 735; 2) ≥ 885
Elongation δ5 (%): 1) ≥ 15; 2) ≥ 12
Area shrinkage ψ (%): 1) ≥ 55; 2) ≥ 50
Impact work Akv (J): 1) ≥ 71; 2) ≥ 55
Hardness: 1) 269~321HB; 2) 311~388HB
Heat treatment specifications and metallographic organization:
Heat treatment specifications: 1) normalizing, 1000~1020; quenching, 1000~1020 oil cooling or air cooling; tempering, 600~710 oil cooling or air cooling; 2) normalizing, 1000~1020, quenching, 1000~1020 oil cooling or Air-cooled; tempered, 540~600 oil-cooled or air-cooled.
Metallographic organization: The tissue is characterized by martensite type.
Delivery status: Generally delivered in the state of heat treatment specification, the type of heat treatment is indicated in the contract; if not specified, it is delivered according to the state without heat treatment.
YB675-73 "Technical conditions for stainless steel and heat-resistant steel bars for aviation";
HB5270-83 "Advanced high quality stainless steel rod for aero-engine rotating parts";
YB677-71 "Aerial stainless steel cold rolled sheet steel";
HB5204-77 "Structural steel, stainless steel and heat-resistant steel forgings"